Dental and Medical Problems
2017, vol. 54, nr 2, April-June, p. 155–160
Publication type: original article
Bond strength of a resin composite to MTA at various time intervals and with different adhesive strategies
Wytrzymałość połączenia żywicy kompozytowej z MTA w różnych przedziałach czasowych i po odmiennym sposobie użycia systemu wiążącego
1 Department of Conservative Dentistry, Chair of Conservative Dentistry and Endodontics, Medical University of Lodz, Łódź, Poland
2 Academic Materials Testing Laboratory, Medical University of Lodz, Łódź, Poland
Background. MTA cannot be used as a single restorative material due to poor esthetics and mechanical properties. Resin-based composite is often placed on top of MTA. Optimal time of doing that and the most effective bonding strategy have not been clearly determined.
Objectives. The aim of the study was to evaluate the bond strength of a composite to MTA at various time intervals and with different adhesive strategies.
Material and Methods. Composite material was bonded to MTA after different time intervals: directly after the placement of MTA (group I), after 24 h (group II), after 72 h (group III). Each group was divided into 2 subgroups (n = 15) in which a universal bonding system was used respectively: in subgroups A as a total-etch adhesive (TE), in subgroups B as a self-etch (SE). The specimens were subjected to shear bond strength test in a universal testing machine.
Results. Statistically significant differences were observed at all time intervals for both bonding protocols TE/SE. In all groups shear bond strength values were higher when the bonding agent was used as a TE vs SE (statistically significant differences in groups I and III). Group II demonstrated the highest bond strength (TE 6.89 MPa; SE 3.82 MPa), followed by group III (TE 5.19 MPa; SE 2.74 MPa) and group I (TE 1.52 MPa; SE 0.74 MPa) where the bond strength was the lowest.
Conclusion. The shear bond strength of composite to MTA depends on both – time interval between MTA placement and the application of an adhesive system and on the bonding strategy. The highest bond strength was obtained when the adhesive was used after 24 h in a total-etch technique.
shear bond strength, composite materials, MTA, adhesive systems
wytrzymałość połączenia na ścinanie, materiały kompozytowe, MTA, systemy adhezyjne
- Darvell BW, Wu RCT. “MTA” – an hydraulic silicate cement: Review update and setting reaction. Dent Mater. 2011;27:407–422.
- Torabinejad M, Parirokh M. Mineral trioxide aggregate: A comprehensive literature review – part II: Leakage and biocompatibility investigations. J Endod. 2010;36:190–202.
- Lee SJ, Monsef M, Torabinejad M. Sealing ability of a mineral trioxide aggregate for repair of lateral root perforations. J Endod. 1993;19:541–544.
- Torabinejad M, Watson TF, Pitt Ford TR. Sealing ability of mineral trioxide aggregate when used as a root end filling material. J Endod. 1993;19:591–595.
- Haapasalo M, Parhar M, Huang X, Wei X, Lin J, Shen Y. Clinical use of bioceramic materials. Endod Topics. 2015;32:97–117.
- Budig CG, Eleazer PD. In vitro comparison of the setting of dry ProRoot® MTA by moisture absorbed through the root. J Endod. 2008;34:712–714.
- Kayahan MB, Nekoofar MH, Kazandağ M, et al. Effect of acid-etching procedure on selected physical properties of mineral trioxide aggregate. Int Endod J. 2009;42:1004–1014.
- Atabek D, Sillelioğlu H, Ölmez A. Bond strength of adhesive systems to mineral trioxide aggregate with different time intervals. J Endod. 2012;38:1288–1292.
- Neelakantan P, Grotra D, Subbarao CV, Garcia-Godoy F. The shear bond strength of resin-based composite to white mineral trioxide aggregate. J Am Dent Assoc. 2012;143:e40–e45.
- Tsujimoto M, Tsujimoto Y, Ookubo A, et al. Timing for composite resin placement on mineral trioxide aggregate. J Endod. 2013;39:1167–1170.
- Tunç ES, Sönmez IS, Bayrak S, Eğilmez T. The evaluation of bond strength of a composite and a compomer to white mineral trioxide aggregate with two different bonding systems. J Endod. 2008;34:603–605.
- Torabinejad M, White DJ. Tooth filling material and method of use. United States Patent. 1995. 5415547.
- Shen Y, Peng B, Ma J, Haapasalo M. What do different tests tell about the mechanical and biological properties of bioceramic materials? Endod Topics. 2015;32:47–85.
- Jaberi-Ansari Z, Mahdilou M, Ahmadyar M, Asgary S. Bond strength of composite resin to pulp capping biomaterials after application of three different bonding systems. J Dent Res Dent Clin Dent Prospects. 2013;7:152–156.
- Thanaratikul B, Santiwong B, Harnirattisai C. Self-etch or etch-and-rinse mode did not affect the microshear bond strength of a universal adhesive to primary dentin. Dent Mater J. 2016;35:174-179.
- Vanderweele RA, Schwartz SA, Beeson TJ. Effect of blood contamination on retention characteristics of MTA when mixed with different liquids. J Endod. 2006;32:421–424.
- Bodanezi A, Carvalho N, Silva D, et al. Immediate and delayed solubility of mineral trioxide aggregate and Portland cement. J Appl Oral Sci. 2008;16:127–131.
- Hara AT, Pimenta LAF, Rodrigues Jr AL. Influence of cross-head speed on resin-dentin shear bond strength. Dent Mater. 2001;17:165–169.
- de Abreu CW, Duarte Filho G, Kojima AN, Jóias RM, Mesquita AMM. Evaluation of crosshead speed influence on shear bond strength test. Braz Dent Sci. 2014;17:50–53.
- Oskoee SS, Kimyai S, Bahari M, Motahari P, Eghbal MJ, Asgary S. Comparison of shear bond strength of calcium-enriched mixture cement and mineral trioxide aggregate to composite resin. J Contemp Dent Pract. 2011;12:457–462.
- Ajami AA, Navimipour EJ, Oskoee SS, Kahnamoui MA, Lotfi M, Daneshpooy M. Comparison of shear bond strength of resin-modified glass ionomer and composite resin to three pulp capping agents. J Dent Res Dent Clin Dent Prospects. 2013;7:164–168.
- Bayrak Ş, Tunç EŞ, Şaroglu I, Eğilmez T. Shear bond strengths of different adhesive systems to white mineral trioxide aggregate. Dent Mater J. 2009;28:62–67.
- Braga RR, Meira JB, Boaro LC, Xavier TA. Adhesion to tooth structure: a critical review of “macro” test methods. Dent Mater. 2010;26:e38–e49.
- Sultan H, Kelly JR, Kazemi RB. Investigating failure behavior and origins under supposed “shear bond” loading. Dent Mater. 2015;31:807–813.